HAL Id: hal-02539969
Submitted on 10 Apr 2020
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Playing with the p-Doping Mechanism to Lower the
Carbon Loading in n-Type Insertion Organic Electrodes:
First Feasibility Study with Binder-Free Composite
Alia Jouhara, Nicolas Dupre, Dominique Guyomard, Alae Eddine Lakraychi,
Franck Dolhem, Philippe Poizot
To cite this version:
Alia Jouhara, Nicolas Dupre, Dominique Guyomard, Alae Eddine Lakraychi, Franck Dolhem, et al..
Playing with the p-Doping Mechanism to Lower the Carbon Loading in n-Type Insertion Organic
Electrodes: First Feasibility Study with Binder-Free Composite Electrodes. Journal of The
Elec-trochemical Society, ElecElec-trochemical Society, 2020, 167 (7), pp.070540. �10.1149/1945-7111/ab7c6d�.
Playing with the p-Doping Mechanism to Lower the Carbon Loading in
n-Type Insertion Organic Electrodes: First Feasibility Study with
Binder-Free Composite Electrodes
To cite this article: Alia Jouhara et al 2020 J. Electrochem. Soc. 167 070540
View the article online for updates and enhancements.
Playing with the p-Doping Mechanism to Lower the Carbon
Loading in n-Type Insertion Organic Electrodes: First Feasibility
Study with Binder-Free Composite Electrodes
Alae Eddine Lakraychi,2
and Philippe Poizot1,z
Université de Nantes, CNRS, Institut des Matériaux Jean Rouxel, IMN, F-44000 Nantes, France
2Institut de la Matière Condensée et des Nanosciences (IMCN), Université catholique de Louvain, 1348 Louvain-la-Neuve, Belgium
3Laboratoire de Glycochimie, des Antimicrobiens et des Agroressources (LG2A), UMR CNRS 7378, Université de Picardie Jules Verne, 80039 Amiens Cedex, France
Organic electrode materials should offer promising alternative to traditional inorganic compounds thanks to several attractive assets such as low-cost, low environmental footprint or the versatility in terms of cell assemblies (cationic and/or anionic shuttling). However, improvements are needed to push forward organic solid electrodes. In particular, decrease the quantity of conductive carbon in the composite electrode is important because it impedes the resulting energy density values. Herein, we present an innovative approach aiming at replacing most of the carbon conductive additive by an electron-conductive anion-inserting crystallized organic material, namely dilithium 2,5-(dianilino)terephthalate (Li2DAnT). Combined with an appropriate n-type lithiated organic electrode material, we demonstrate the beneﬁcial effect of adding Li2DAnT (23 wt%)/carbon (10 wt%) compared to a typical conducting carbon loading of 33 wt% for powder-based composite electrodes made without binder by simple mixing and grinding with a pestle in a mortar. In fact, Li2DAnT provides an efﬁcient percolating conductive network and contributes to the overall reversible capacity of the composite electrode through its own storage properties.
© 2020 The Author(s). Published on behalf of The Electrochemical Society by IOP Publishing Limited. This is an open access article distributed under the terms of the Creative Commons Attribution Non-Commercial No Derivatives 4.0 License (CC BY-NC-ND,http://creativecommons.org/licenses/by-nc-nd/4.0/), which permits non-commercial reuse, distribution, and reproduction in any medium, provided the original work is not changed in any way and is properly cited. For permission for commercial reuse, please email:email@example.com. [DOI:10.1149/1945-7111/ab7c6d]
Manuscript submitted December 26, 2019; revised manuscript received February 28, 2020. Published March 19, 2020.This paper is part of the JES Focus Issue on Challenges in Novel Electrolytes, Organic Materials, and Innovative Chemistries for Batteries in Honor of Michel Armand.
Supplementary material for this article is availableonline
Commercially available rechargeable batteries, especially Li-based cells, may face some limitations in the near future due to the major use of scarce chemical elements (e.g., 3d transition metals) in their manufacture. In addition, the question about their potential environmental impact throughout their entire life cycle is posed considering the context of their expected massive and widespread development.1,2 For example, a recent compilation of life cycle assessment (LCA) analyses performed on commercial Li-ion bat-teries (LIBs) has highlighted that a cumulative energy demand of 328 kWh is needed across all chemistries to produce 1 kWh of stored electrochemical energy together with the greenhouse gas (GHG) emissions of 110 gCO2eq.
Moreover, such LCA data were obtained at the manufacturing outlet (“cradle-to-gate analyses”) meaning they do not take into account both collection and recycling steps while other eco indicators such as human toxicity (HTP) are not considered. This situation calls for developing new and efﬁcient battery chemistries easier to recycle for an affordable price and based on more abundant resources if we want to pursue the progress of our technology-oriented societies.
One possible alternative to inorganic materials lies in the development of redox-active organic materials for which the literature on the topic has been expanding since the last decade after years of silence.2,4–10 Twenty years ago, M. Armand and co-workers11pointed out the interest of some redox-active hybrid organic materials to reach speciﬁc capacities higher than 500 mAh g−1 while Nishide’s group demonstrated in the early 2000s high electron-transfer kinetics with nitroxide polymer electrodes.12,13 Based on the assembly of the most abundant chemical elements on the Earth, organic chemistry provides also great opportunities for discovering innovative electrode functionalities thanks to molecular
engineering together with access to two electrochemical storage mechanisms10,14,15: “n-type” electrode reactions that involve an ionic compensation with cation release upon oxidation and “p-type” electrodes reactions that imply an anion uptake. Furthermore, they can be used in non-aqueous as well as in aqueous media16–18 including in the solubilized state for redox-ﬂow battery applications, for which demonstrators are in progress.19,20However, for applica-tions as solid organic electrodes, improvements are needed espe-cially to increase the energy density of organic-based electrodes, which are often impeded by substantial carbon contents in the electrode formulation.4–9For comparison, the amount of conducting carbon in commercial Li-based batteries is less than 5%–10% of the total mass of the electrode and generally more than 20% with most organic electrodes reported in the literature. Although it should be recognized that organic compounds are often insulators6 some options exist to overcome the problem of electronic conductivity such as favoring molecular backbones with extended electron delocalization or the decrease of the particle size.
For example, we have recently demonstrated that formulation optimization based on a processing solvent in which not only the binder but also the organic active material is soluble (controlled recrystallization process) gives rise to 86% retention of the rever-sible Li insertion in Indigo Carmine (IC) based electrodes over 50 cycles at C/10 rate with 10 wt% carbon only.21On the other hand, it is also known that some organic compounds can replace carbon when semiconducting properties appear thanks to overlap of π-orbitals, generally after p-doping. Replacing carbon by different conducting organics has already been tested with conventional inorganic electrode materials such as LiFePO4 or Si.
Basically, intrinsically conducting polymers (CPs) such as polyani-line (Pani)25,26constitute the most common examples. Inspired by this property, Sjödin and co-workers27have fabricated theﬁrst all-organic proton batteries which require no conductive additives by combining redox-active pendant groups to π-conjugated p-doped zE-mail:firstname.lastname@example.org
*Electrochemical Society Member.
polymer backbone, resulting in so-called conducting redox polymers (CRPs). Another type of non-polymeric example is the nearly planar delocalized π-electrons (n-type) tetra-lithium perylene-3,4,9,10-tet-racarboxylate salt (PTCLi4) that can achieve good electrochemical
performance as negative electrode with only 0.5 wt% carbon nanotubes (12.0 mg cm−2, 1.2 mAh cm−2) probably due to the long-range aromatic–aromatic interactions (π-stacking) within the crystal structure.28S. Lee et al.29 have also recently demonstrated that the charge-transfer complex phenazine –7,7,8,8-tetracyanoqui-nodimethane (PNZ–TCNQ) can be cycled vs Li with only 2.5 wt% of carbon by due to its well-known intrinsic conducting properties but at 50% of the theoretical capacity. Lastly, we pinpointed few years ago that the p-type crystallized lithiated salt of 2,5-(dianilino) terephthalate (Li2DAnT), which derives from the phenyl-capped
aniline dimer, can cycle without carbon because the reversible anion ingress into the layered Li2DAnT induces a huge change of the
electrode conductivity like observed during the p-doping of Pani.30,31
Within this background and inspired by the works of both Deng et al.32and Huang et al.33on the partial replacement of conducting carbon by CPs to cycle n-type organic active materials (i.e., perylene-3,4,9,10-tetracharbonxydiimide (PTCDI)-doped polypyr-role and Na2C6O6-doped Pani, respectively), we have tried for the
ﬁrst time to implement this approach with a non-polymeric conducting agent by choosing Li2DAnT. Indeed, this crystallized
lamellar compound34displays several assets. First, it can deliver a stable capacity of about 75 mAh g−1(Fig. S1 is available online at stacks.iop.org/JES/167/070540/mmedia) by reversible one-electron reaction with concomitant anion ingress.30Second, it exhibits electronic conductive properties similarly to polyaniline.31Third, it can be considered as a sustainable chemical because the acid precursor (namely 2,5-(dianilino)terephthalic acid or “anilic acid”) is now produced by Clariant International Ltd. from“bio-succinic acid” (renewable raw compound); the anilic acid being a key intermediate in the large scale synthesis of red and violet quinacri-done pigments.35
To rapidly demonstrate the macroscopic efﬁciency of Li2DAnT
as electroactive and electronic conducting agent, two n-type lithiated positive organic electrode materials have been selected for the benchmark (dilithium (2,5-dilithium-oxy)-terephthalate, namely Li4-p-DHT and tetralithium 2,5-dihydroxy-1,4-benzenedisulfonate,
namely Li4-p-DHBDS, Fig. S1) for which the corresponding
composite electrodes have been prepared without any binder or optimized formulation, but rather through simple grinding of organic powders (Li4-p-DHT–Li2DAnT or Li4-p-DHBDS–Li2DAnT) with
low amounts of conducting carbon. Interesting electrode perfor-mance has been obtained with the Li4-p-DHT–Li2DAnT blend due
to the good compatibility of their respective electroactive potential window.
Chemicals.—Reagents were purchased from commercial sources and used without further puriﬁcation: 2,5-dihydroxyterephthalic acid H4-p-DHT (Sigma Aldrich, ⩾98.0%), 2,5-(dianilino)terephthalic
acid (Clariant), lithium hydride (Alfa Aesar), lithium methoxide (2.2 M in methanol) (Sigma Aldrich,⩾98.0%). Lithium perchlorate (battery grade), N,N-dimethylformamide, methanol and diethylether solvents were anhydrous and purchased from Aldrich whereas propylene carbonate (PC, battery grade) was obtained from Novolyte. All synthetic reactions were conducted inside an argon-ﬁlled glove box (MBRAUN) containing less than 1 ppm of dioxygen and water (T= 30 °C).
Analytical techniques.—Infrared spectra were recorded on a FTIR Bruker Vertex 70. Air-free pellets were prepared in glove box by mixing the sample with spectroscopic-grade potassium bromide at 1 wt%.1H and13C liquid NMR spectra were recorded on a Bruker AVANCE III 400 MHz. Chemical shifts (δ) are given in ppm
relative to tetramethylsilane (TMS). Deuterium oxide was purchased from Sigma Aldrich (purity higher than 99.5%). The thermogravi-metry (TG)-Mass spectrothermogravi-metry (MS) coupled experiments were carried out with a STA449F3 Jupiter and QMS403C Aëolos instruments from NETZSCH under argon at a heating rate of 5 °C min−1up to 800 °C. Scanning electron microscopy (SEM) investi-gations were performed on a JSM-7600F from JEOL. X-ray diffraction (XRD) patterns were recorded at room temperature with a Bruker D8 Advance powder diffractometer. Data were collected in the Bragg-Brentano geometry with a Cu-anode X-ray source operated at 40 kV and 40 mA.
Materials synthesis.— Synthesis of dilithium (2,5-dilithium-oxy)-terephthalate (Li4-p-DHT).—The synthesis procedure was
pre-viously reported by Chen’s group.36Into a homogeneous solution of H4-p-DHT (1.0 g, 5.1 mmol, 1 eq.) in anhydrous methanol (50 ml)
was dripped 10.1 ml of lithium methoxide (2.2 M in methanol, 22.4 mmol, 4.4 eq.). A yellow precipitate was formed after≈3 min under stirring at room temperature. After reaction for 40 h, the as-prepared solid wasﬁltered and washed (3 × 6 ml) with anhydrous methanol, and dried under vacuum at 100 °C overnight. The ﬁnal compound Li4-p-DHT was obtained by thermal treatment at 220 °C
for 24 h in a drying glass oven (Büchi B-585 glassoven for drying) in glovebox to afford Li4-p-DHT as orange powder (yield: 87%). The
desolvation effectiveness was checked by thermal analysis and the absence of MeOH traces in NMR and IR spectra. IR (KBr pellet, cm−1) 1570 (νas COO−), 1467–1412 (ν C=C), 1363 (νs COO−),
1232 (ν CO−Li ), 880-800 (ν C−H);1H NMR (400 MHz, D2O)δ
(ppm) 7.11 (2H, s);13C NMR (100 MHz, D2O)δ (ppm) 175.97 (C,
C=O), 152.78 (C, C−O−), 125.39 (C, C−COO−), 118.82 (C, C −H).
Synthesis of tetralithium 2,5-dihydroxy-1,4-benzenedisulfonate (Li4-p-DHBDS).—The chemical route to synthesize this salt has
been previously reported by our group.37In short, the lithiation of 2,5-dihydroxy-1,4-benzenedisulfonic acid (1.311 g, 4.85 mmol, 1 eq.) is performed in anhydrous N,N-dimethylformamide (50 ml) with a stoichiometric amount of lithium hydride (154.0 mg, 19.4 mmol, 4 eq.). A white precipitate was formed under stirring at room temperature. After reaction for 48 h, the prepared solid was collected by centrifugation, washed 3 times with diethyl ether and dried in vacuum at 60 °C for 3 h. The observations of the as-obtained powder by SEM shows aggregates of particles with acicular morphology (Fig. S2a). The ﬁnal Li4-p-DHBDS was obtained in
82% yield after heating in drying glass oven at 300 °C overnight. The desolvation effectiveness was checked by thermal analysis and the absence of DMF traces in NMR and IR spectra. IR (KBr pellet, cm−1) 1452 (ν C=C), 1440 (ν SO3−), 1208 (ν C−O), 850 (δ O−Li ); 1 H NMR (400 MHz, D2O) δ (ppm) 7.03 (2 H, s); 13 C NMR (100 MHz, D2O) δ (ppm) 151.04 (C, C−O−), 132.85 (C, C−SO3−), 118.35 (C, C−H).
Synthesis of dilithium 2,5-(dianilino)terephthalate (Li2DAnT)
.—The lithiation of 2,5-(dianilino)terephthalic acid was adapted from a procedure previously described by our group.30In practice, 2,5-(dianilino)terephthalic acid (1.689 g, 4.85 mmol, 1 eq.) were mixed with a stoichiometric amount of lithium hydride (77.0 mg, 9.7 mmol, 2 eq.) in anhydrous N,N-dimethylformamide (50 ml). A pale yellow precipitate was formed under magnetic stirring at room temperature. After reaction for 48 h, the prepared solid was collected by centrifugation, washed 3 times with diethyl ether and dried in vacuum at 60 °C for 3 h. The platelet morphology of the as-prepared particles observed by SEM imaging (Fig. S2b) combined with the strong Bragg peak observed at 6.5° on the powder XRD pattern (Fig. S3) conﬁrm the lamellar structure of the as-obtained compound.30 The ﬁnal Li2DAnT was obtained in 85% yield after thermal
treatment in a drying glass oven at 250 °C overnight. The desolva-tion effectiveness was checked by thermal analysis and the absence of DMF traces in NMR and IR spectra (Fig. S4). IR (KBr pellet,
cm−1) 3370 (ν N−H), 1600 (νasCOO−), 1570-1500 (ν C=C), 1440 (νs COO−), 1280 (ν C−N), 550 (δ COO−Li ); 1 H NMR (D2O, 400 MHz)δ (ppm) 7.75 (2H, s), 7.44-7.40 (4H, m, H-meta), 7.26-7.24 (4H, m, H-ortho), 7.07-7.10 (2H, m, H-para);13C NMR (D2O, 100 MHz)δ (ppm) 175.1 (C, C=O), 151.0 (C, C−NH), 136.2 (C, C −NHPh), 129.6 (CH, C-meta), 128.4 (C, C−COOLi), 121.5 (CH), 120.7 (CH, C-para), 118.6 (CH, C-ortho).
Electrochemical measurements.—The electrochemical testing of the composite electrode materials was performed in Swagelok®-type cells using a Li metal disc as the negative electrode and a Whatman® separator soaked with LiClO4 1 M in PC as the
electrolyte (V ≈ 400 μl); the perchlorate anion giving the best electrochemical performance towards Li2DAnT.
The composite powder-based electrodes based on the Li4-p-DHT–Li2DAnT or
Li4-p-DHBDS–Li2DAnT mixtures were prepared in an argon-ﬁlled
glovebox by grindingﬁrst (with a pestle in a mortar, batch of 30 mg) the two organic materials during 2 min. Then the conducting carbon (Ketjenblack EC-600JD, AkzoNobel) was added to the mixture and grinded again for 2 min more. The as-obtained mixtures were directly transferred into the cell (mtotal= 6 mg, 5.3 mg cm−2, Fig.
S5) then cycled in galvanostatic mode using a MPG-2 multi-channel system (Bio-Logic SAS, Seyssinet-Pariset, France). Electrochemical Impedance Spectroscopy (EIS) measurements were performed as previously reported31 by using a home-made Swagelok®-type 3-electrode cell connected to a VMP3 instrument (Bio-Logic SAS). The reference electrode consisted of a ring of Li metal surrounding the working electrode, whereas a Li metal disc was used as a negative electrode. The typical amplitude of the sinusoidal voltage signal used was 7 mV for frequency values ranging from 200 kHz to 10 mHz. Measurements have been performed after a relaxation period to ensure a sufﬁcient stability of the potential (dE/dt < 10 mV h−1).
Results and Discussion
On the contrary of our previous formulation optimization21 aiming to fabricate low-carbon IC-based electrode tapes for which an original aqueous processing has been developed (including a controlled recrystallization of IC with carboxymethylcellulose so-dium salt), no complex formulation of a slurry was intentionally performed in the present study. The carbon additive was simply grinded with the blend of organic materials (Li4-p-DHT–Li2DAnT
or Li4-p-DHBDS–Li2DAnT) without binder. This extremely simple
procedure has been known and applied for decades when using Swagelok-type cells.38–40It offers the advantage to rapidly probe the electrochemical performance of an electroactive material despite a non-optimized shaping of the electrode. Herein, our intention was to macroscopically demonstrate the beneﬁcial effect of Li2DAnT as
both electrochemically active and non-polymeric conducting com-ponent when preparing composite electrodes in non-optimized and raw conditions.
Theﬁrst tested system was the blend based on Li4-p-DHT as the
active n-type material because this compound is known to be highly reversible with good energy efﬁciency when cycled in the 2.2–3.4 V vs Li+/Li potential range.41 Note that the second electron is never observed in our experimental conditions14,41 (Fig. S1a) on the contrary of the procedure reported by Chen’s group,36 which is based on a complex nanostructuration of this organic compound. Several ratios were tested but rapidly promising results were obtained with amounts of carbon adding as low as 10 wt% despite the extreme simplicity of the as-prepared composite electrodes. Therefore, we will discussﬁrst on the electrochemical data obtained with the best blend that consists in Li4-p-DHT (67 wt%)/Li2DAnT
(23 wt%)/carbon (10 wt%), denoted“Blend (67/23/10 wt%).” It is worth noting that the total amount of conducting carbon corresponds to 33% in mass that is the typical carbon ratio used in our former studies.41–43
Figure1a shows the potential-speciﬁc capacity traces relative to the composite electrode made of the blend (3 representative cycles in black), together with theﬁrst cycle in red of a composite electrode based on Li4-p-DHT/carbon (67/33 wt%) for the sake of comparison.
As expected the blend shows an efﬁcient reversible delithiation/ lithiation process demonstrating again the high stability of this lithiated organic electrode material when cycled in carbonate-based liquid electrolyte. Compared to the typical electrochemical feature of the Li4-p-DHT/carbon composite electrodes (red curve), a capacity
gain is observed that can be ascribed to the shoulders located within the 3.2–3.4 V vs Li+/Li potential range. In order to better analyze such respective electrochemical traces measured in galvanostatic mode, Fig.1b show the corresponding incremental capacity curve obtained for the composite electrode made of the blend super-imposed with the trace for both Li4-p-DHT/carbon and
Li2DAnT/carbon composite electrodes in red and blue, respectively.
Unambiguously, the capacity observed above 3.1 V vs Li+/Li is related to the reversible perchlorate insertion in the Li2DAnT host
structure (one-electron reaction within the considered potential window) to form the corresponding radical cation (Fig. S1c). But the most striking feature is that with only 10 wt% of conducting carbon, the composite electrode made of the Li4-p-DHT–Li2DAnT
blend exhibits very good capacity retention upon cycling with only 6% of capacity fading after 50 cycles while the adding of 33 wt% of conducting carbon leads to lower performances after 250 cycles (Fig.2). The speciﬁc capacity evolution for the composite electrode based on Li4-p-DHT/carbon (90/10 wt%) is also presented as control
experiment for comparison purpose (Fig.2). Although quite stable upon cycling, the as-observed speciﬁc capacity is lower of about 33% indicating that 10 wt% of carbon additive cannot provide a sufﬁciently efﬁcient percolating conductive network. Note that an additional capability test was performed after the 50th cycle by successively applying cycling rates of 1 Li+/5 h, 1 Li+/2 h, 1 Li+/1 h for 6 cycles. The collected data show that the composite electrode made of the blend (67/23/10 wt%) can sustain a stable capacity of 95 mAh g−1at the highest applied current conﬁrming that the material can handle slow to fast charge-discharge reactions without being damaged or degraded. In addition, Fig.3shows the electrochemical performances of another blend still at 10 wt% of carbon but containing a lower amount of Li4-p-DHT (45 wt% only vs 67 wt
%) combined with Li2DAnT at the same ratio (denoted“Blend (45/
45/10 wt%)”). As expected, the measured reversible capacity per gram of Li4-p-DHT is higher due to the noticeable contribution of
the electroactivity of Li2DAnT to the total capacity (Fig.3a). But the
most important result is that good capacity retention can also be observed upon cycling despite the high (macroscopic)“dilution” of Li4-p-DHT into the composite powder electrode, which contains
only 10 wt% of conducting carbon. This experiment reinforces the above conclusions about the efﬁcient percolating conductive net-work provided by Li2DAnT.
To go further, EIS analyses were performed to analyze the interface resistance at different state of charge/discharge during the ﬁrst cycle of both the best blend (67/23/10 wt%) and the composite electrode based on Li4-p-DHT/carbon (90/10 wt%) for comparison
purpose (Fig.4). Nyquist diagrams for the two powder composite electrodes exhibit systematically well-deﬁned semi-circles at higher frequencies, which is a typical behavior characterizing the charge transfer resistance in combination with the double layer capacitance. All the diagrams exhibit also the characteristic linear Warburg region at low frequencies corresponding to the diffusion of species inside the material following their transfer at its surface. Interestingly, the characteristic frequencies related to the respective semi-circles are very similar which can suggest the probing of the same limiting phenomenon and presumably the charge transfer resistance of Li4-p-DHT. Although only a slight increase of
impedance is observed in both cases upon cycling, one can observe that the resistance values are lower (by a factor 2) in the case of Li4-p-DHT/carbon (90/10 wt%) mixture compared to the blend (67/
23/10 wt%). Nevertheless, the corresponding galvanostatic curves Journal of The Electrochemical Society, 2020 167 070540
show that less than half of the practical capacity (of one exchanged electron per Li4-p-DHT unit) is obtained for the (90/10 wt%)
composite powder electrode (Fig.4d) whereas the full capacity is reached with the blend (67/23/10 wt%) (Fig. 4a). Otherwise, the average polarization value corresponding to the lithium removal/ uptake mechanism in Li4-p-DHT appears very similar in both cases (
i.e., ΔE ≈ 160 mV). If these low polarization values suggest an efﬁcient percolating network in the two composite electrodes, the fact that the capacity of the electrode containing Li4-p-DHT/carbon
(90/10 wt%) is severely limited indicates the powder composite electrode is macroscopically not homogenous and that 10 wt% of carbon additive is not sufﬁcient to provide electronic connection to all the active material particles. It can be estimated that only half of the particles seems connected to the percolation network giving rise to a ratio closer to 80/20 rather than the expected 90/10 in agreement with the lower measured impedance in this case. To sum up, despite the raw conditions used in the present study to prepare the composite
electrodes based on Li4-p-DHT, our different electrochemical
measurements converge to a positive contribution of the electro-active Li2DAnT material to the electronic percolating network.
The second system tested was based on the Li4-p-DHBDS–Li2DAnT couple. Compared to Li4-p-DHT, the
disulfonate counterpart is known to react at higher average potentials (i.e., <E > ≈ 3.2 V vs Li+/Li against 2.55 V for Li4-p-DHT)
according to the expected two-electron reaction (Fig. S1b). The appropriate potential range for its cycling is between 2.5 and 4.0 V vs Li+/Li as previously reported.37 The Li4-p-DHBDS active
material displays however lower electrochemical performance than Li4-p-DHT upon cycling such as a noticeable charge/discharge
potential difference (polarization of about 300 mV) and an irrever-sible capacity of 20% after theﬁrst cycle. Several ratios were also tested but larger amounts of Li2DAnT was then considered to be
added with Li4-p-DHBDS because this material appears less
con-ductive than Li4-p-DHT.37 In practice, the following ratio was
selected: Li4-p-DHBDS (42 wt%)/Li2DAnT (48 wt%)/carbon (10 wt
%), denoted“Blend (42/48/10 wt%).” Figure5a shows the potential-capacity proﬁle of the Li2DAnT−Li4-DHBDS blend
galvanostati-cally cycled vs Li at a rate of 1 Li+/10 h together with the typical ﬁrst cycle of the Li4-DHBDS/carbon composite electrode for the
sake of comparison. In addition, Fig. 5b shows the corresponding incremental capacity curves for their respectiveﬁrst cycle to better grasp the electrochemical steps occurring in the two composite electrodes. Theﬁrst charge is roughly characterized by a progressive potential increase before to reach aﬁrst plateau located at 3.3 V vs Li+/Li followed by another one at 3.4 V as previously observed with Li4-p-DHBDS/carbon (67/33 wt%) composite electrode (Fig.5a, red
trace). Then, a last plateau appears at 3.6 V corresponding to the second anion insertion into Li2DAnT.30 Note that this
electroche-mical step was not visible in Figs.1a,b because the reverse anodic potential was limited to 3.4 V. Finally, the measured capacity after the complete charge is about 250 mAh per gram of Li4-p-DHBDS,
exceeding its theoretical capacity due to the 2-electron reaction involved in Li2DAnT. With this second example, it is demonstrated
again that only 10 wt% of conducting carbon allow access to the full capacity of the electroactive Li4-p-DHBDS material. The
electro-chemical feature of the subsequent discharge curve is ﬁrst char-acterized by the reversible reactivity of Li2DAnT with an obvious
plateau at 3.5 V corresponding to the extraction of the second anion from the host structure. Then the discharge curve shows quite
Figure 1. (a) Potential-speciﬁc capacity curves for the composite electrode based on Li4-p-DHT made of the blend (67/23/10 wt%) for cycles no. 1, 2, and 25 (in black) together with theﬁrst cycle (in red) of a composite electrode based on Li4-p-DHT/carbon (67/33 wt%) acquired in galvanostatic mode at a rate of 1 Li+ exchanged per mol of Li4-p-DHT in 10 h (1 Li+/10 h, Im= 12.1 mA g−1). The green circle indicates the starting open circuit potential. (b) Overlay of potential vs incremental capacity dQ/dE curves (1st cycle) for the composite electrode made of the blend (in black) and Li4-p-DHT/carbon 67/33 wt% (in red), respectively. For comparison, the typical trace for a composite electrode made of Li2DAnT/carbon (67/33 wt%) is shown in blue.
Figure 2. Capacity retention curves (in discharge) with coulombic ef ﬁ-ciency for the composite electrode based on Li4-p-DHT made of the blend (67/23/10 wt%) in black, Li4-p-DHT/carbon (67/33 wt%) in red, and Li4-p-DHT/carbon (90/10 wt%) in pink as control experiment. Note that a capability test was integrated after the 50th cycle by successively applying higher cycling rates for 6 cycles:1 Li+/5 h (24.2 mA g−1), 1 Li+/2 h (60.2 mA g−1), 1 Li+/1 h (103.9 mA g−1). Note that 250 cycles correspond to about 180 days in operation.
different electrochemical behaviors compared to the expected trace for Li4-p-DHBDS (Fig.5a, red trace). In short, a series of successive
electrochemical steps is observed instead of the occurrence a unique potential plateau at about 3 V (more visible in Fig.5b) giving rise to a recovered capacity of only 190 mAh g−1 (irreversibility: 24%). Unfortunately, the subsequent cycles show poor stability with large
capacity loss. This capacity fading is attributed here to the exfolia-tion phenomenon of the zwitterionic form of Li2DAnT obtained at
3.6 V vs Li+/Li after the insertion of two anions per DAnT moiety (Fig. S1c) and the subsequent loss of electronic conductivity initially provided by Li2DAnT.
This assumption is well supported by the disappearance of the high-potential plateau related to the second
Figure 3. (a) Potential-speciﬁc capacity curves for the composite electrode based on Li4-p-DHT made of the blend (45/45/10 wt%) for cycles no. 1, 2, 5, and 25 (in black). (b) Corresponding capacity retention curves (in discharge) together with coulombic efﬁciency.
Figure 4. First galvanostatic charge/discharge curve measured in a home-made Swagelok®-type 3-electrode cell and corresponding points (with color) where EIS measurements were performed for (a) the best blend (67/23/10 wt%) based on Li4-p-DHT and the composite electrode based on Li4-p-DHT/carbon (90/10 wt %), respectively (reference and counter electrodes: Li; electrolyte: LiClO41 M in PC). (b), (d) Corresponding Nyquist diagrams.
insertion process occurring in Li2DAnT. Another cell was cycled
within the 2.8–3.5 V potential range to restrict the exfoliation process. A better stability upon cycling was then observed however the compatibility between the two electroactive materials Li4-p-DHBDS/Li2DAnT remains limited.
To sum up, the strong contrast in terms of electrochemical performance when comparing Li4-p-DHBDS and Li4-p-DHT in
presence of Li2DAnT shows that this p-type redox-active lamellar
structure could be useful as both electroactive and electronic percolating additive but at the condition to applied a cut-off potential below 3.5 V vs Li+/Li in order to suppress the poorly reversible second anion insertion. Therefore, one can anticipate that the coupling of Li2DAnT with other n-type material working within a
suitable potential window such as Li4-o-DHT (2.85 V vs Li+/Li)43
should provide good electrochemical performances too. Conclusions
Inspired by recent publications showing that the addition of p-type conductive polymers to n-p-type organic electrode materials could potentially replace the large carbon addition, we have investigated the properties of the p-type (non-polymeric) Li2DAnT
material as a“smart” and sustainable additive. Having previously established that this compound was able to reversibly intercalate anions and become electronic conductive,30,31composite electrodes based on either Li4-p-DHT–Li2DAnT or Li4-p-DHBDS–Li2DAnT
mixtures grinded with 10 wt% carbon only were electrochemically assessed in Li half-cell. Despite the raw conditions used in the present study to prepare the composite electrodes (simple powder grinding without binder), we demonstrate in the case of Li4-p-DHT
that the 2-D Li2DAnT structure could efﬁciently replace the carbon
additive limiting therefore the dead mass of the composite electrode thanks to its faradaic contribution to the reversible capacity by anion insertion/deinsertion. Nevertheless, poor electrochemical perfor-mances were obtained when using the Li4-p-DHBDS–Li2DAnT
blend notably due to the overall 2-electron reaction occurring in Li2DAnT that induces exfoliation of its lamellar structure and
subsequent degradation of the composite electrode. Hence the excellent electrochemical performance of Li4-p-DHT–Li2DAnT
blend is attributed to the stability and conductivity of Li2DAnT in
the 2.2–3.4 V vs Li+/Li potential range. Mixing Li2DAnT with other
compatible redox active materials should behave similarly.
This work funded by the University of Nantes. The authors wish specially to thank M. Armand from CIC Energigune (Spain) for the collaborative works in organic batteries, the laboratory CEISAM (UMR CNRS 6230) in Nantes for complementary experiments as well as S. Ohren (Clariant International Ltd., Switzerland) for providing 2,5-(dianilino)terephthalic acid (“anilic acid”) and support to this research.
Philippe Poizot https://orcid.org/0000-0003-1865-4902 References
1. P. Poizot and F. Dolhem,Energy Environ. Sci., 4, 2003 (2011).
2. P. Poizot, J. Gaubicher, S. Renault, L. Dubois, Y. Liang, and Y. Yao,Chem. Rev., In Press.
3. J. F. Peters, M. Baumann, B. Zimmermann, J. Braun, and M. Weil,Renew. Sustain. Energy Rev., 67, 491 (2017).
4. Y. Liang, Z. Tao, and J. Chen,Adv. Energy Mater., 2, 742 (2012). 5. Z. Song and H. Zhou,Energy Environ. Sci., 6, 2280 (2013).
6. B. Häupler, A. Wild, and U. S. Schubert,Adv. Energy Mater., 5, 1402034 (2015). 7. T. B. Schon, B. T. McAllister, P. F. Li, and D. S. Seferos,Chem. Soc. Rev., 45,
8. S. Lee, G. Kwon, K. Ku, K. Yoon, S. K. Jung, H. D. Lim, and K. Kang,Adv.
Mater., 30, 1704682 (2018).
9. Y. Liang and Y. Yao,Joule, 2, 1690 (2018).
10. P. Poizot, F. Dolhem, and J. Gaubicher,Curr. Opin. Electrochem., 9, 70 (2018).
11. N. Ravet, C. Michot, and M. Armand,MRS Proc., 496 (1997).
12. H. Nishide, S. Iwasa, Y. J. Pu, T. Suga, K. Nakahara, and M. Satoh,Electrochim. Acta, 50, 827 (2004).
13. T. Suga, Y. J. Pu, K. Oyaizu, and H. Nishide,Bull. Chem. Soc. Jpn., 77, 2203 (2004).
14. A. Jouhara, N. Dupré, A. C. Gaillot, D. Guyomard, F. Dolhem, and P. Poizot,Nat. Commun., 9 (2018).
15. A. Jouhara, E. Quarez, F. Dolhem, M. Armand, N. Dupré, and P. Poizot,Angew.
Chem. Int. Ed., 58, 15680 (2019).
16. K. Hatakeyama-Sato, H. Wakamatsu, R. Katagiri, K. Oyaizu, and H. Nishide,Adv. Mater., 30, 1800900 (2018).
17. S. Perticarari, T. Doizy, P. Soudan, C. Ewels, C. Latouche, D. Guyomard, F. Odebel, P. Poizot, and J. Gaubicher,Adv. Energy Mater., 9, 1803688 (2019). 18. S. Perticarari et al.,Chem. Mater., 31, 1869 (2019).
19. X. Wei et al.,ACS Energy Lett., 2, 2187 (2017).
20. W. Liu, W. Lu, H. Zhang, and X. Li,Chem. - Eur. J., 25, 1649 (2019). 21. E. Deunf, P. Poizot, and B. Lestriez,J. Electrochem. Soc., 166, A747 (2019).
22. Q. Wang, N. Evans, S. M. Zakeeruddin, I. Exnar, and M. Grätzel,J. Am. Chem.
Soc., 129, 3163 (2007).
23. G. Liu, S. Xun, N. Vukmirovic, X. Song, P. Olalde-Velasco, H. Zheng, V. S. Battaglia, L. Wang, and W. Yang,Adv. Mater., 23, 4679 (2011).
Figure 5. (a) Potential-speciﬁc capacity curves for the composite electrode based on Li4-p-DHBDS made of the blend 42/48/10 wt%’ for cycles no. 1, 2, and 5 (in black) together with theﬁrst cycle (in red) of a composite electrode based on Li4-p-DHBDS/carbon (67/33 wt%) acquired in galvanostatic mode at a rate of 1 Li+exchanged per mol of Li4-p-DHBDS in 10 h (1 Li+/10 h). The green circle indicates the starting open circuit potential. (b) Overlay of potential vs incremental capacity dQ/dE curves (1st cycle) for the composite electrode based on Li4-p-DHBDS made of the blend (42/48/10 wt%) in black, Li4-p-DHBDS/carbon (67/33 wt%) in red, and Li2DAnT/carbon (67/33 wt%) in blue.
24. P. Sengodu and A. D. Deshmukh,RSC Adv., 5, 42109 (2015).
25. E. M. Geniès, A. Boyle, M. Lapkowski, and C. Tsintavis,Synth. Met., 36, 139 (1990).
26. P. Novák, K. Müller, K. S. V. Santhanam, and O. Haas,Chem. Rev., 97, 207 (1997). 27. R. Emanuelsson, M. Sterby, M. Strømme, and M. Sjödin,J. Am. Chem. Soc., 139,
28. A. Iordache, D. Bresser, S. Solan, M. Retegan, M. Bardet, J. Skrzypski, L. Picard, L. Dubois, and T. Gutel,Adv. Sustain. Syst., 1, 1600032 (2017).
29. S. Lee et al.,Energy Storage Mater., 20, 462 (2019).
30. E. Deunf, P. Moreau, E. Quarez, D. Guyomard, F. Dolhem, and P. Poizot,J. Mater. Chem. A, 4, 6131 (2016).
31. E. Deunf, N. Dupré, E. Quarez, P. Soudan, D. Guyomard, F. Dolhem, and P. Poizot,
CrystEngComm, 18, 6076 (2016).
32. W. W. Deng, Y. F. Shen, X. M. Liang, J. W. Feng, and H. X. Yang,Electrochim. Acta, 147, 426 (2014).
33. Y. Huang, G. Jiang, J. Xiong, C. Yang, Q. Ai, H. Wu, and S. Yuan,Appl. Surf. Sci., 499, 143849 (2020).
34. E. Quarez, E. Deunf, V. Cadiou, T. Gutel, F. Boucher, D. Guyomard, and P. Poizot,
CrystEngComm, 19, 6787 (2017).
35. High Performance Pigments, Clariant webpage, https://clariant.com/en/Business-Units/Pigments/Coatings/Quinacridonelast accessed December 2019.
36. S. Wang, L. Wang, K. Zhang, Z. Zhu, Z. Tao, and J. Chen,Nano Lett., 13, 4404 (2013).
37. A. E. Lakraychi, E. Deunf, K. Fahsi, P. Jimenez, J. P. Bonnet, F. Djedaini-Pilard, M. Bécuwe, P. Poizot, and F. Dolhem,J. Mater. Chem. A, 6, 19182 (2018). 38. E. Wang, J. M. Tarascon, and S. Colson,J. Electrochem. Soc., 138, 166 (1991). 39. J. M. Tarascon and D. Guyomard,J. Electrochem. Soc., 138, 2864 (1991). 40. P. Poizot, S. Laruelle, S. Grugeon, L. Dupont, and J.-M. Tarascon,Nature, 407, 496
41. S. Renault, S. Gottis, A. L. Barrès, M. Courty, O. Chauvet, F. Dohlem, and P. Poizot,Energy Environ. Sci., 6, 2124 (2013).
42. S. Renault, J. Geng, F. Dolhem, and P. Poizot,Chem. Commun., 47, 2414 (2011). 43. S. Gottis, A. L. Barrès, F. Dolhem, and P. Poizot,ACS Appl. Mater. Interfaces, 6,